# User:Allison K. Alix/Notebook/Thesis Research/2013/08/13

(Difference between revisions)
Jump to: navigation, search
 Revision as of 13:01, 13 August 2013 (view source) (→Calculations)← Previous diff Revision as of 13:34, 13 August 2013 (view source) (→DNA Attachment)Next diff → Line 46: Line 46: ==DNA Attachment== ==DNA Attachment== - 1) Mix 300uL AuNP@SiO2 with 30uL APS and 470uL 100% ethanol. Sonicate for 30 minutes + 1) Mix 1mL 5nM AuNP@SiO2 with 5uL 1mM APS. Stir for 1hr. + + 2) Reduce thiol DNA to HS-DNA using DTT. Mix 3mL 3uM DNA with 2mg Sulfo-SMCC in 2mL 0.05M KP buffer

## Revision as of 13:34, 13 August 2013

Project name Main project page
Previous entry      Next entry

## Scaled up Silica-Coating Procedure

Original: 1mL AuNP & MHA solution/2μL TES/0.125mL NH4OH/5mL 2-propanol

1) Re-scale to use 9mL AuNP/MHA solution

New: 9mL AuNP&MHA solution/18uL TES/1.125mL NH4OH/45mL 2-propanol

2) Stir solutions for one hour to allow reaction to proceed

3) Centrifuge solutions at 4000 rpm for one hour

4) Re-suspend particles in water

## Calculations

Original concentration of AuNP/MHA solution is 4.7nM

4.7nM(9mL)=55.143mL(x)

x= 0.767nM

0.767x10^-9moles/L x 1L/1000mL x 36mL = 2.7612 x 10^-11 moles AuNP total

2.7612 x 10^-11 moles AuNP x 6.02 x 10^23 particles/mole = 1.66 x 10^13 total Au nanoparticles

• We want a 5nM solution

5x10^-9 moles/L x 1L/1000mL x 6.02x10^23 particles/mole = 3.01 x 10^12 particles/mL

1.66 x 10^13 particles / x = 3.01 x10^12 particles/1 mL

x = 5.52mL

Dilute AuNP in 5.52mL water after removing supernantant

5.52mL/24 vials = 230uL per vial.

## DNA Attachment

1) Mix 1mL 5nM AuNP@SiO2 with 5uL 1mM APS. Stir for 1hr.

2) Reduce thiol DNA to HS-DNA using DTT. Mix 3mL 3uM DNA with 2mg Sulfo-SMCC in 2mL 0.05M KP buffer